Survey

* Your assessment is very important for improving the work of artificial intelligence, which forms the content of this project

Document related concepts

Transcript

PHYSICAL RE VIEW B VO LUME Photovoltaic effect and interband Department 12, NUM BK R 12 magneto-oytical 15 DE C EMBER 1975 transitions in InP P. Rochon and E. Fortin of Physics, University of Ottawa, Ottawa, Canada (Received 20 January 1975) A study is made of the oscillatory spectral distribution of the photovoltaic (PV) effect of a gold-indium phosphide Schottky barrier in magnetic fields of up to 70 kG. Spectra are obtained for both the direct and wavelength-modulated PV signals, the latter being compared to the wavelength-modulated reflectivity data. The spectra are taken at 4.2 K in the Faraday configuration for both circular polarizations. The transition energies associated with the spectral oscillations are corrected for exciton-binding effects, and are analyzed as Landau levels in terms of the Pidgeon and Brown coupled-bands theory of interband magnetoabsorption. The fit to the data gives a conduction-band effective mass m, 0.079 +0.001 and Luttinger parameters 5. 15 ~0.05, y, 0.94~0.03, and y3 —1.62~0, 03. The direct observation of the split-off valence-bandy& to-conduction-band transition gives 60=0.108+0.003 eV and an approximate effective mass of msoiNlp — = — /~ = =0.21+0.02. I. INTRODUCTION The study of interband magneto-optical transitions has been extensively used in order to determine accurate band parameters for many semiconductors. The theory for the quantization of electronic levels in a magnetic field was first developed by Landau. ' It was refined by Luttinger and Kohn to include valence-band degeneracy and further refined by Pidgeon and Brown to include the nonparabolicity of the conduction band. However, in interband magneto-optics, one can only use the latter theory directly in cases where the exciton contributions to the spectra are negligible. Exciton effects can be included by using the theories developed by Elliott and Loudon, and more recently by Altarelli and Lipari. 6'~ The problem of the exciton in a magnetic field has been solved for the cases of low and high fields (i. e. , y«1 and y»1, where y=h&o, /280, the ratio of the cyclotron energy to the exciton binding energy). No explicit solution for degenerate nonparabolic bands at intermediate fields has yet been presented. The determination of the band parameters of indium phosphide through magneto-optics presents both experimental and theoretical difficulties. Due to the relatively high effective masses involved, high magnetic fields are required to produce observable energy quantization, and even at 70 kG only the transitions from the light-hole valence band will produce any observable effects, these effects being small in comparison to the background. The exciton contributions to the spectrum are large because of the exciton's large binding energy; thus the observed quantum oscillations must be corrected for these effects. The correction in the case of indium phosphide is difficult to perform explicitly since the field involved is in the intermediate region (y —1). In order to circumvent the problems of excitonic participation, the data presented below are empirically corrected for the exciton contributions by a method used by Vrehen for QaAs. The data were obtained by using the photovoltaic effect which has recently been used with some success in interband magneto-optics. ' This method was used for detection because of its high signalto-noise ratio and its experimental simplicity, and also because it can be easily coupled to wavelength modulation to obtain the first derivative of the observed signal directly. In the following paragraphs a brief review of the theory of the effects involved and used here is presented, followed by a description of the experimental setup and a discussion of the results. The data are analyzed and fitted to the Pidgeon and Brown theory for I.andau levels. The parameters obtained from the fit are used to analyze the energy shift of the transition from the split-off valence band to the conduction band (hereafter referred to as S.O. ). II. THEORY A. Photovoltaic effect The open-circuit zero-bias photovoltage V„ across an illuminated Schottky barrier can be shown 11 to be V'„= (kT/e)ln(J/Jo+ 1), where Jo is the equilibrium dark-current density in the semiconductor and is the nonequilibrium current density caused by the illumination. In the case of a metal-semiconductor junction where the contribution to the photocurrent from the semi- J 5803 transparent metal film can be ignored, current is given by /=ed (1 —e ), the photo- where P is the quantum efficiency, N is the number of photons crossing the film yer unit area, 0. is the absorption coefficient of the semiconductor, and W is the thickness of the space-charge region, mhich in the case of an abrupt junction is approximately given by (2e, y, /eX, )'", (3) semiHere &~ is the effective permittivity of the conductor, Qs is the barrier height, and No is the W= ' density of 3.onlzed donors. %Shen oTV & &, changes in the absorption coefficient will give rise to changes in the photocurrent and thus in turn to changes in the photovoltage. For example, when oW&1 Eq. (2) reduces to sociated with each Landau level. The theory of the behavior of excitons in a magnetic field has been developed for the cases of low and high magnetic fields. ~ Unfortunately in the intermediate-field region (y= 1, the case of InP here) the theory has yet to be explicitly developed. In order to circumvent this difficulty, the experimental data can be empirically corrected using the method suggested by prehen. This correction involves shifting the experimental points to higher energies by R(H)/ (2s+ 1}, whel e R(P) ls the binding energy of the exciton associated with the first Landau level as a function of magnetic field, arid n is the Landaulevel quantum number. The value of R(Jf} can be obtained by taking the difference between the experimental data for the first exciton level and the approximately calculated position of the first Landau level. The nem data are then fitted to the PidgeonBrown. theory. III. EXPERIMENTAI. 4p, ~ (1/o, ) 4o, , (6) Thus, in order to observe changes in the absorption coefficient of a semiconductor due to an imposed external magnetic field, the sample must be selected in such a may that the condition O.W & 1 is satisfied. For a given case, this can be accomplished by selecting the parameters P~ and No of Eq. (3). 8. Magneto-optics Interband magneto-optical effects usually observed in absorption or reQectivity spectra can thus be displayed, in the proper circumstances, in the spectral distribution of the photovoltaic effect and such spectra can be analyzed to give band parameters of the semiconductor. The PtLdgeonBrown theory for interband magneto-optical transitions is to date the most realistic theory for the displacement of the Landau-level-associated transitions as a function of magnetic field. The theory takes into account the valence-band degeneracy as mell as the interaction between the valence bands, conduction band, and the upper bands. Thus a fit to the experimental transition energies gives the approximate functional parameters of the theox'y. The experimental results, homever, include contributions not only from Landau-like transitions but also reflect the participation of excitons as- The samples are obtained from a monocrystalline block of n-type InP with a room-temyerature impurity concentration of 2x 10 cm, 3. This material should be yure enough to obey the condition a&v &1 (where &o is the cyclotron frequency and ~ the relaxation time), necessary for the observation of magneto-optical structure associated with the light-hole valence-band- to- conduction-band transitions. At the same time the impurity concentration should be sufficient to satisfy the barrier width condition, as mell as to provide a moderate electric field at the junction. This material seemed to satisfy all the conditions, since quantum oscillations were observed and no Franz-Keldysch effect could be observed at 4. 2 K. A rough estimate, assuming the ionized-impurity concentration at 4. 2 K to be of the order of 10 cm 3, with and Qs = 0. 56 V, gives the barrier e~ = 12. 09, midth 9 =5x10 cm, with a maximum electric field of E= 2x 10~ V/cm at the barrier. The samyles mere polished mith A1393 powder, etched in a methanol 10-vol. gB rsolutio nan dkept in an inert atmosphere or high vacuum during the remainder of the preparation in order to minimize surface oxidation and the resultant changes in the spectrum. The contacts on the photovoltaic samples were ylaced in a "sandwich" configuration, the back contact being made by evaporating indium and alloying in a nitrogen-atmosphere furnace at 300 C, and the front contact consisting of an evaporated semitransparent gold film. The samples mere mounted in the Faraday configuration in such a manner that S((B[( )[E, where S is the incident-radiation propagation vector, B the magnetic field, and E the junction electric field. (Note E l(B in order to avoid crossed-field effects. ) ' %%u (ill) E FFEC T AND INTERBAND. PHOTOVOLTAIC InP T = 4.2 I Ex ~ ei «III» K FIG. 1. WavelengthreQ ectivity (hR/R) and wavelengthmod ulated photovoltaic g V») effect near the 1$ exciton line: solid line, 4V» experimental; dashed line, bR/R fit; ~, b, R/R experimental. Oi of II modulated I ~ S .. I) Is l I ~O I l.420 ENERGY (sV) These samples were placed in an indeyendent cham- ber within a suyerconducting magnet and kept at 4. 2 K by a He exchange gas at a pressure of 10 TOLT, The optical system consisted of a &-m grating monochromator mounted in a double-beam geometry and coupled to an HR polarizer and a Fresnel rhomb, thus providing monochromatic radiation circularly polarized at better than 90% over the spectral range of interest. The beam was chopped at 85 Hz and synchronous detection was used The wavelength modulation was prothroughout. vided by a vibrating refractor plate placed in the monochromator. A low-noise silicon photodiode (EG and G type HAD-1000) was used as detector in order to obtain the ref lectivity data. A more complete descriytion of the apparatus elsewhere. 4 can be found IV. RESULTS AND DISCUSSION A. Comparison of wavelength-modulated photovoltaic effect and wavelength-modulated reflectivity In order to establish the correspondence between the structures seen in the photovoltaic spectra and the pertinent transition energies, a comparison was made between the photovoltaic derivative spectrum and the modulated-ref lectivity spectrum. ref lectivity Qn Fig. 1, the wavelength-modulated b, R/R near the 1S exciton line at 1.4183 ep is presented together with the wavelength-modulated photovoltaic spectrum 6 V„. The ref lectivity curve FORT IN ROC HON AND XPO v O " ir 'I )P r P XTO l l lP 9 l I I l l liI i I I I I I I I I I l l I I l I B= 7OI \J I % Lop l g l I l II S I ~ II II TH 5c QE gE where A xs an exciton e a 0.82 0. 8l =0 A=0 0. 6 and thee (p. ~) form" 5e I I I 0.85 WAVE„E o, 87 4R 8 I l was fitted to th e G I I l 0.88 teions Inp I l h' al. I I ..'"t'" eterA. was ' Ql in jmum w he zero , found too be g parameter eory, was found to gy which urve js AR/8 curv o the 4'' ally can be mea- ccuracy. ' iFIQ. 3. Spectraal distrirect-phototr' ) szgvo so s RS S associate d wave- d, I I ] cr a point whi 1 I e e noted thaa the exc t correspond 1 I ' (&) roadening T e, br o I orentzian lu d ex dielectrric consta t, e „e {LCP) light ansi sg t Th are l Rb d Rs in Tab]e g I I Rted pho- . cUl Rrl y- pol„d fo»eft--cjr I I (g, .gnal and tovoltaic its corrrespondin g Moda] . (g~ ~) refle t. vyy + signal at R ~Rgnetlc f ' of 7o kQ Ji 8 ia, Spectr Rl PIG hot jon f l ated photovol- I I / rw I l / I I l Sr I %s r~ Jv x IO,~i I O. 88 0.87 TIO I l O. 86 I 0.85 I 0 84 0. NGTH l O. 82 ()Lr. m) left- ar y-polar i ansitions are ig b t, T ignal at 55 kQ G for l 0.8 I PHOTOVOLTAIC E F FEC T AND INTERBAND. .. 5807 tnP I. 52, — 8 Il S II T=4. 2 &ill& K RCP FIG. 4. Energy positions of the spectral oscillations as functions of the magnetic field for right-circularlypolarized {RCP) light. The e& l. 46 lines represent theoretical transitions labeled as in Table II. Only the points .of line 7-10 were used in the ~l' ~ 0 fit. 4 0~ l. 4'5 I. 42— 0 —o —e—o — —— I I I I I0 20 50 40 MAGNETIC ~ 4 I 1 I 50 60 70 FIELD (k G} The complete spectra of r R/R and 4 V„at 70 ko a, re presented for comparison in Fig. 2. The transition-energy positions (labeled as in Table II below) which were taken as data, are indicated on the figure. It is noted that in the case of the Landau-like oscillations having a large broadening parameter, the maxima of the hP~, curves corresponded with the minima for the hR/R curves to within 0. 5 meV, which is as good as the resolution of the apparatus. A major difficulty in using only the LR/R data is that the reflectivity signal was very weak and noisy, in contrast to that of the photovoltage. This is clearly demonstrated on Fig. 2 by the high visibility of the 8. 0. transition in the b, P„spectrum in comparison with that of the LR/R spectrum Thus, fo. r each magnetic-field value and polarization, the accumulated data consisted of the data from the b. R/R spectra, from the 6 V~, spectra as well as from the direct photo- voltaic (V„) spectra. Figure 3 presents a comparison of the direct photovoltaic syectrum and its associated wavelength-modulated 6 V~, spectrum at 55 kG for leftcircularly-polarized light. The transitions are seen in the direct spectrum as very small oscillations, even when the signal is amplified and offset; these oscillations, however, are quite evident in the modulated spectrum. B. Landau-level analysis The energies of the oscillations seen in the spectra are plotted as functions of the magnetic field in Figs. 4 and 5 for right- and left-circularlypolarized light, resyectively. Following Vrehen, it was assumed that the binding energy of the excitons associated with Landau levels of higher quantum numbers (e. g. , n= 4, 5, 6) is negligible when compared to the experimental resolution (- 0. 5 ' P. 5808 ROC HON AND E. FORTIN 55— 1. InP !.52 8 II V =O. 8 Z II ~Ill& K LCP l.50 49— l. FIG. 5. Energy positions of the spectral oscillations as functions of the magnetic field for left-circularlypolarized light. The lines represent theoretical transitions labeled as in Table Q. Only the points of lines 7-9 were used in the fit. 4 1.47 C9 K m 1.46 K Ld 1.45 14+ 1.4'5 l. 42— 0 ~ 4 ~ I I I 20 30 40 MAGNETI C 4 ~ 4— ~ —~ I 50 60 70 FIE LD (k G) meV). Thus these three levels for both polarizations were simultaneously fitted to the PidgeonThe Brown theory for I.andau-level transitions. fit was done by a convergence program which iterates with respect to the conduction-band effective mass and the Luttinger parameters y& and ya. Other parameters necessary to the fit were obtained as follows: (a) The band-gap value E~ = 1.423 eV was obtained from the zero-field convergence point of the three upper curves of both polarizations. energy 6= 0. 108 eV (b) The spin-orbit-splitting was obtained directly from the spectra at B = 0. (c) The higher-band interaction parameter f= 0. 0 was obtained by minimizing the rms error of the fit with respect to this parameter. (d) The anisotropy factor (y~ —y~~) was taken from Lawaetz. ~ (e) The value of K~ is approximately given by I 2 & =V3+s L Vp —s & L VZ —s- The fit produced the band parameters presented in Table I, where parameters such as m„, and E~ are calculated using the approximate equations of Aggarwal The p.arameters obtained differ somewhat from theoretical values; however, they are in agreement with the latest experimental values obtained by cyclotron resonance; for example, m, h/ma= 0. 12 of Leotin et al. and m, /mo = 0. 0803 of Chamberlain et al. ' The theoretical lines produced in Figs. 4 and 5 are derived from the parameters obtained in the fit and are identified in Table II. The lines are labeled according to the Pidgeon-Brown notation in the case of Landau levels; in the case of exciton levels, the lines are labeled as the corresponding Landau level [which is R(H)/(2n+ 1) eV above the exciton level]. For example, in the right-circu- g„g PHOTOVOLTAIC 12 TABLE I. Comparison of the band parameters determined in the present experiment with the theoretical values and other experimental values. Parameter Present work Theory 1.423+0. 0005 eV 1.42 eVa O. 13 ev' 0. 108 + 0. 002 e V 17 +1 0, 079 + 0. 001 ~L pL m, gmo m~/m0 m o/nZO ZL O. 11b 5. 15~0. 05 0. 94+ 0. 03 1.62+0. 03 0. 12 + 0. 01 0. 45+ 0. 05 0, 21 +0. 01 0, 12 +0. 03 1.48+0. 05 —1. 90+0. 05 0. 5 meV Reference 17. "Reference 18. 'Reference 19. O. OSO, ' O. 072d .. 5809 TABLE II. Identification of the quantum oscillations. The notation used is as in the Pidgeon and Brown. Q, ef. 4) scheme. In the table the transitions are identified as Landau levels {L) or as exciton states (Ex) associated with the pertinent Landau level. For n&4 the experimental resolution does not allow the differentiation between a Landau 1evel and its associated exciton. 16 RGP -2. O' p, o+0, 2 ~L 20. 4 eVa Experiment 1.424+ O. OO1' E FFECT AND INTERBAND. 0. 0803 No. 1 2 3 4 6. 28a 2. 08 2. 76' O. OS9, ' O. OS6d 0 12c 0. 85, 0 50 0. 60 0, 1700, 184 1.47a LGP Notation Type a'(1) O.s(0) Ex L a (1) 0.'({)) a'(1) nc(0) a+(2) ec(1) b'(2) P'(1) 5 6 a'(3) a'(4) a'(5) '(6) a'(7) 7 8 9 10 Number L? ExP LY L'P 0; (2) uc(3) L, L, L, L, ~'(4) &c(5) &'(6) Notation Type b'(o) P'0. ) b {0) P'(1) b'(0) Pc(1) a'(1) O.c(2) a'(2) 0. (3) Ex L b Ex Ex Ex Ex LV L'P L'P Exl L, Ex L, Ex L, Ex (2) Pc(3) b'(3) P'(4) b'(4) P'(5) b'(5) P'(6) l. 20a "Reference 20. Reference 21. =1.4237 eV, essentially the value deducted from the extrapolated Landau levels. D. Spin-orbit transitionwnergy shift Because of the observed spectral width of the the exact energy positions of such transitions were limited to a resolution of approximately 1 meV. It was thus difficult to observe dif- S. O. transition, data both the I.andau transition (line 8) and its associated exciton level (line 1) are seen. The higher-quantum-number lines (4, 5, 6) are an unresolved mixture of Landau and associated exciton levels. At low quantum numbers, due to the admixture of a number of possible Landau transitions and associated exciton levels, the exact identity of data was difficult to establish. Thus, among the possible overlapping theoretical lines, the line which best described the data was chosen as the label. larly-yolarized a'(1)a'(0) InP T=4.2K S II 8 II&III& theory C. Exciton parameters In zero magnetic field, the exciton position is found to be E„=1.4183+ 0. 0002 eV, which agrees with the values of Evangelisti et al. ~ (1.4185) and White et al. (1.4182). Using the expression developed by Baldereschi and Lipari ' for the exciton-reduced effective mass together with the band parameters of Table I we obtain p, o/ma=(mo/m, +yg) I) 5 e 4 I E CI 3 =0. 056 . In turn using /2eri'»' gives R,„=5.2+0. 1 meV, a value which compares favorably with that of Evangilisti et af. (4. 8 meV) and White et al. (4. 9 meV). The binding energy of the exciton and its position at zero field thus give the band-gap value of E~ IO I I 20 30 I I 40 50 MAGNETIC ~ 60 I 70 FIELD (k G) FIG. 6. Energy shift of the split-off to conductionband transition as a function of the magnetic field. The points represent the averages of both polarizations; the line is a theoretical fit using the parameters of Table I ' (present work). P. 5810 ROCHON AND ferences between the left- and right-circularlypolarized spectral positions of the transition at a given magnetic field„A general energy shift as a function of magnetic field was, however, observed and is presented in Fig. 6. The points here represent the average shifts in energy of both polarizations. The theoretical line shown in Fig. 6 is given by n, E = —,' (mo/m, —mo/m„)S(B), which is a first-order approximation for. the shift in the S. O. transition. In this equation the values m, /m 0= 0. OVQ and m „/m 0 = 0. 21 (from Table I, yresent work) were used. The function S(g) is given by E. The above study of the interband magneto-optical properties of InP has shown that the photovoltaic effect and its wavelength derivative can be powerful methods for observing very small changes in the optical properties of semiconductors. These methods can be especially useful in the infrared where the usual ref lectivity and absorption measurements are sometimes difficult due to the lack of suitable detectors. In the case of InP, further investigation at low and intermediate fields should prove useful in determining more precisely the effects of exciton participation. It may then be possible to study the exciton's behavior in the light of the recent theoretical developments of Altarelli and Lipari ' and of and thus set al. . ACKNOWLEDGMENTS The agreement of the data to the fit again increases our confidence in the parameter derived from the Landau-level analysis, specifically the values of m„yz~, m„. ~L. D. Landau, Z. Phys. 64, 629 (1930). B. Lax and J. G. Mavroides, in Semiconductors and Semimetals, edited by R. K. Willardson and A. C. Beer (Academic, New York, 1972), Vol. 3, p. 326. 3J. M. Luttinger and W. Eohn, Phys. Rev. 97, 869 (1965). C. R. Pidgeon and R. Brown, Phys. Bev. 146, 575 (1966). R. J. Elliott and B. Loudon, J. Phys. Chem. Solids 15, 196 (1960). M, Altarelli and N. O. Lipari, Phys. Rev. B 7, 3798 (1973). 7M. Altarelli and O. Lipari, Phys. Rev. B 9, 1733 (1e74). Q. H. F. Vrehen, J. Phys. Chem. Solids 29, 129 (1968). P. Bochon and E. Fortin, Can. J, Phys. 52, 1173 {1974). N. A. Belov, Kim Gacan De, O. V. Kosogov, and M. A. Mazanzina, Fiz. Tech. Poluprovodn. 7, 2179 (1973) [Sov. Phys. Semicond. 7, 1451 (1974)]. ~ S. M. Sze, I'hysies of Semiconductor Devices (Wiley, New York, 1969), p. 363, 2W. J. Turner, W. E. Reese, and R. S. Pettit, Phys. Rev. 136, A67 (1964). A. Barbaric and E. Fortin, J. Phys. Chem. Solids 35, 1521 (1974). ~4A. FQion and E. Fortin, Phys. Bev. B 8, 3852 (1973). ¹ ¹ M. Cardona, Modulation 12 V. CONCLUSION Cho 8(P) =8kB/moc FORTIN Spectroscopy (Academic, New The authors wish to thank K. S. Song and R. C. Smith for valuable discussions on this work. This research was supported by the National Research Council of Canada. York, 1969), p. 110. B. Senechal and J. C. Woolley, Phys. Bev. Lett. 27, 1563 (1e71). ~P. Lawaetz, Phys. Rev. B 4, 3460 (1971). J. U. Fishback, G. Benz, Stath, and M. H. Pilkuhn, Solid State Commun. 11, 725 (1972). 9J. Leotin, B. Barbaste, S, Ashenazy, M. S. Skolnick, B. A. Stradling, and J. Tuckendler, Solid State Commun. 15, 693 {1974). 20M. Cardona, J. Phys. Chem. Solids 24, 1543 (1963); M. Cardona, J. Phys. Chem. Solids 26, 1351 (1965). ~'J. M. Chamberlain, P. E. Simmonds, B. A. Stradling, and C. C. Bradley, Proceedings of the Eleventh International Conference on Semiconductors, Warsaw, 1972 (unpublished), p. 1016. 2 R. L. Aggarwal, in Semiconductors and Semimetals, edited by R. K. Wil1, ardson and A. C. Beer (Academic, New York, 1972}, Vol. 9. F. Evangelisti, J. U. Fishback, and A. Frova, Phys. Rev. B 9, 1516 O. e74). 4A. M. White, P. J. Dean, L. L. Taylor, R. C. Clarke, D. J. Ashen, J. B. Mullin, and P. D. Greene, J. Phys. C 5, 1727 (1972). 25A. Baldereschi and N. O. Lipari, Phys. Rev. B 3, 439 GB. ¹ (1971). 26K. Cho, S. Sugu, W. Dreybrodt, Phys. Rev. B 11, 1512 (1975), and F. Willmann,